Influence of different welding processes on the mechanical
Influence of different welding processes on the mechanical properties of structural steel S960MC
Institute of Materials Science and Welding, University of Technology Graz, Austria
voestalpine Stahl GmbH, Linz, Austria
Kapfenberg, Austria 4Fronius International GmbH, Wels, Austria
The use of high strength low alloyed (HSLA)
structural steels, such as S960MC, is constantly
increasing in engineering industry today. Typical
applications are structures in load handling,
transportation vehicles and lifting equipment such
as telescoping booms and cranes. The higher
strength of the material offers increased payload
and/or reduced weight of structures compared to
standard structural steel [1, 2].
Welding of HSLA steel however, is more demanding
since the process window of heat input and cooling
rate is smaller. It has been proven that this steel
can be welded succesfully with suitable welding
methods, such as laser beam, laser-hybrid or
modern gas metal arc welding. Also the filler metals
play an important role in the welding of HSLA
steels [3, 4].
The focus of this work is to study the influence of
different welding methods and filler materials on the
mechanical properties of S960MC welds.
voestalpine Böhler Welding GmbH,
Materials and Methods
8 mm thick sheets of structural steel S960MC were used for the welding experiments (Tab.3). Basic mechanical
properties and chemical composition are given in Tables 1 and 2.
Table 1: Chemical Composition of S960MC in wt%
Table 2: Mechanical properties of S960MC
Table 3: Weld Seam Geometry, Number of Passes, Heat Input and t8/5 times for all examined welding processes
4, 7.5, 11
The standard DIN EN 10025-6  requires that welded joints of S960MC steel
have a tensile strength in the range of 980 MPa to 1150 MPa. All joints, which
were welded with the 960 IG filler metal, break in the base material and therefore
fullfill the specification. Of all the welds that were welded with EMK 8 only the LH
welds always break in the base material. Alltough two of the three plasma welds
break in the weld metal, they still reach the necessary strength limit. The TIG and
GMA welds show a significant drop in both yield- and tensile strength and cannot
meet the requirements.
Figure 1: Yield and tensile strength of LH-, P-, TIG-, and GMA welds of S960MC
steel using EMK 8 (left) and 960 IG (right) filler metal.
DIN EN ISO 10025-6 also requires an impact toughness of at least 30 J at −20 ◦C in
the heat affected zone as well as in the weld metal. With the exception of the TIG
welds using 960 IG all joints fulfill this specification (Fig. 1). The impact toughness
in the weld metal of the EMK 8 welds increases with decreasing energy density of
the welding process. This can also be correlated to the increasing strength of the
joints. No trend regarding energy density of the process can be seen for the 960 IG
Figure 2: Impact toughness of LH-, P-, TIG-, and GMA welds of S960MC steel in
the HAZ (top) and WM (bottom) for EMK 8 (left) and 960 IG (right).
It could be shown that it is possible to weld 8 mm thick S960MC sheets using different filler metal and different welding techniques. 5 out of 8 tested combinations,
LHW+EMK 8, LHW+960 IG, PW+EMK 8, PW+960 IG and GMAW+960 IG, fulfill the requirements stated by DIN EN ISO 10025-6.
The use of undermatching filler material, i.e. EMK 8 is possible when welding with high power and power density welding techniques like laserhybrid- or plasma beam
welding, which offers an economic benefit.
For TIG and GMA welding undermatching with EMK 8 is not sufficient since the weld metal does not reach the neceassary strength level.
The filler metal 960 IG produces sound welds for all tested welding techniques with the exception of the TIG joints. These fail the standard due to their lack of impact
toughness in the weld metal.
P. Zimmer, “Zur Bewertung der Kaltrisssicherheit von Schweißverbindungen aus hochfesten Feinkornbaustählen,” PhD thesis, 2007, isbn: 9783981165586.
A. NAGAO, T. ITO, and T. OBINATA, “1 100 MPa Class Ultra High Strength Steel Plates with Excellent Toughness and High Resistance to Delayed Fracture for Construction and Industrial Machinery,” JFE Technical Report, vol. 11, no. 11, pp. 13–18, 2008.
I. Bunaziv, “Optimization of parameters for fiber laser-MAG hybrid welding in shipbuilding applications,” PhD thesis, 2013, p. 125.
H. Engström, K. Nilsson, J. Flinkfeldt, T. Nilsson, A. Skirfors, and B. Gustavsson, “Laser Hybrid Welding of High Strength Steels,” in Proc. ICALEO 2001, LIA (Orlando, FL), 2001, pp. 125–134.
DIN EN 10025-6:2011-04, Hot rolled products of structural steels - Part 6: Technical delivery conditions for flat products of high yield strength structural steels in the quenched and tempered conditions, 2011.
General foster notes / Acknowledgment
The K-Project Network of Excellence for Metal JOINing is fostered in the frame of COMET - Competence Centers for Excellent Technologies by BMWFW, BMVIT, FFG, Land Oberösterreich, Land
Steiermark, Land Tirol and SFG. The programme COMET is handled by FFG.